# Electronic Supplementary Material (ESI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2019

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Pr700W625Zn75O3000
_database_code_depnum_ccdc_archive 'CCDC 1894705'
loop_
_audit_author_name
_audit_author_address
'Philippe Lacorre' 'IMMM, UMR 6283 CNRS, Le Mans Universit?, France'
_audit_update_record             
;
2019-01-30 deposited with the CCDC.	2019-03-13 downloaded from the CCDC.
;

_pd_block_id                     Pr7W6.25Zn0.75O30

#=============================================================================

# POWDER DIFFRACTOMETER CHARACTERISTICS : 

_diffrn_measurement_device_type  'PANalytical Empyrean'
_diffrn_radiation_type           'X-ray Cu K\a'
loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
1.54056 1.0000
1.54439 0.5000

_pd_spec_mount_mode              reflection
_pd_meas_scan_method             step

_diffrn_ambient_temperature      300

#=============================================================================

# COMPOUND FORMULATION & CHARACTERISTICS : 

# Formula

_chemical_formula_moiety         'O30 Pr7 W6.25 Zn0.75'
_chemical_formula_sum            'O30 Pr7 W6.25 Zn0.75'
_chemical_formula_weight         2664.36

# Colour

_pd_char_colour                  'light green'


# Density

_exptl_crystal_density_diffrn    7.932

# Symmetry

_symmetry_cell_setting           Trigonal
_symmetry_space_group_name_H-M   'R -3'
_symmetry_space_group_name_Hall  '-R 3'

loop_
_symmetry_equiv_pos_as_xyz
x,y,z
-y,x-y,z
-x+y,-x,z
-x,-y,-z
y,-x+y,-z
x-y,x,-z
x+2/3,y+1/3,z+1/3
-y+2/3,x-y+1/3,z+1/3
-x+y+2/3,-x+1/3,z+1/3
-x+2/3,-y+1/3,-z+1/3
y+2/3,-x+y+1/3,-z+1/3
x-y+2/3,x+1/3,-z+1/3
x+1/3,y+2/3,z+2/3
-y+1/3,x-y+2/3,z+2/3
-x+y+1/3,-x+2/3,z+2/3
-x+1/3,-y+2/3,-z+2/3
y+1/3,-x+y+2/3,-z+2/3
x-y+1/3,x+2/3,-z+2/3

# Cell parameters

_cell_length_a                   16.8427(2)
_cell_length_b                   16.8427(2)
_cell_length_c                   6.8112(1)
_cell_angle_alpha                90.0000
_cell_angle_beta                 90.0000
_cell_angle_gamma                120.000
_cell_volume                     1673.30(3)
_cell_formula_units_Z            3
_cell_measurement_temperature    300

#=============================================================================

# REFINEMENT DATA :

#  Data used in refinement :

_pd_proc_2theta_range_min        9.000
_pd_proc_2theta_range_max        130.000
_pd_proc_2theta_range_inc        0.0131


#  Refinement program and convergence

_computing_structure_refinement  FULLPROF
_refine_ls_shift/su_max          0.01


#  Reliability factors for points with Bragg contributions

_pd_proc_ls_prof_R_factor        10.3
_pd_proc_ls_prof_wR_factor       10.8
_pd_proc_ls_prof_wR_expected     2.57

_refine_ls_R_I_factor            7.79
_refine_ls_goodness_of_fit_all   4.32

#=============================================================================

# ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS :

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_Wyckoff_symbol
_atom_site_thermal_displace_type
_atom_site_B_iso_or_equiv
Pr1 Pr+3 0.0000 0.0000 0.0000 1.000 3 a Biso 0.63(6)
Pr2 Pr+3 0.7791(2) -0.0140(3) 0.3330(8) 1.000 18 f Biso 0.63(6)
Zn1 Zn+2 0.0000 0.0000 0.5000 0.750 3 b Biso 0.31(4)
W1 W+6 0.0000 0.0000 0.5000 0.250 3 b Biso 0.31(4)
W2 W+6 0.1961(2) 0.0124(2) 0.1711(6) 1.000 18 f Biso 0.31(4)
O1 O-2 0.236(2) 0.113(3) 0.317(6) 1.000 18 f Biso 3.1(4)
O2 O-2 0.294(3) 0.040(3) 0.027(6) 1.000 18 f Biso 3.1(4)
O3 O-2 0.170(2) 0.108(2) 0.061(6) 1.000 18 f Biso 3.1(4)
O4 O-2 0.208(3) -0.078(3) 0.291(5) 1.000 18 f Biso 3.1(4)
O5 O-2 0.039(2) 0.117(2) 0.308(5) 1.000 18 f Biso 3.1(4)

_chemical_formula_structural     'Pr Pr6 (Zn0.75W0.25) W6 (O6)5'

#=============================================================================

# DISTANCES AND ANGLES :

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pr1 O3 2.541(10) 1_555
Pr1 O3 2.541(15) 2_555
Pr1 O3 2.541(13) 3_555
Pr1 O3 2.541(10) 4_555
Pr1 O3 2.541(15) 5_555
Pr1 O3 2.541(13) 6_555
Pr1 O5 2.725(11) 1_555
Pr1 O5 2.725(11) 2_555
Pr1 O5 2.725(13) 3_555
Pr1 O5 2.725(11) 4_555
Pr1 O5 2.725(11) 5_555
Pr1 O5 2.725(13) 6_555
Pr2 O1 2.114(12) 2_655
Pr2 O1 2.844(15) 4_656
Pr2 O2 2.677(14) 4_655
Pr2 O2 2.430(19) 11_555
Pr2 O3 2.504(12) 2_655
Pr2 O3 3.434(15) 4_655
Pr2 O4 2.890(15) 3_655
Pr2 O4 2.945(13) 4_656
Pr2 O4 2.408(12) 18_545
Pr2 O5 2.480(16) 2_655
Pr2 O5 3.227(12) 6_656
Zn1 O5 2.177(11) 1_555
Zn1 O5 2.177(11) 2_555
Zn1 O5 2.177(14) 3_555
Zn1 O5 2.177(11) 4_556
Zn1 O5 2.177(11) 5_556
Zn1 O5 2.177(14) 6_556
W1 O5 2.177(11) 1_555
W1 O5 2.177(11) 2_555
W1 O5 2.177(14) 3_555
W1 O5 2.177(11) 4_556
W1 O5 2.177(11) 5_556
W1 O5 2.177(14) 6_556
W2 O1 1.777(15) 1_555
W2 O2 1.770(14) 1_555
W2 O3 2.012(15) 1_555
W2 O3 2.103(12) 5_555
W2 O4 1.827(17) 1_555
W2 O5 1.960(12) 3_555
O1 O2 2.75(2) 1_555
O1 O2 2.745(17) 10_555
O1 O3 2.049(20) 1_555
O1 O4 3.01(2) 1_555
O1 O4 3.007(18) 6_556
O1 O4 3.14(2) 9_555
O1 O5 3.36(2) 1_555
O1 O5 2.609(14) 3_555
O1 O5 3.117(18) 5_556
O2 O1 2.75(2) 1_555
O2 O1 2.745(17) 10_555
O2 O2 3.03(2) 9_555
O2 O2 3.03(2) 14_544
O2 O3 2.84(2) 1_555
O2 O3 2.787(15) 5_555
O2 O4 2.539(17) 1_555
O2 O4 3.099(17) 9_554
O2 O4 3.04(3) 14_544
O3 O1 2.049(20) 1_555
O3 O2 2.84(2) 1_555
O3 O2 2.787(19) 6_555
O3 O3 2.640(18) 5_555
O3 O3 2.64(2) 6_555
O3 O4 3.021(17) 6_555
O3 O5 2.840(19) 1_555
O3 O5 2.738(16) 3_555
O3 O5 2.628(17) 5_555
O4 O1 3.01(2) 1_555
O4 O1 3.007(18) 5_556
O4 O1 3.14(2) 14_544
O4 O2 2.539(17) 1_555
O4 O2 3.041(17) 9_555
O4 O2 3.099(19) 14_545
O4 O3 3.021(20) 5_555
O4 O4 2.643(19) 16_545
O4 O5 2.58(2) 3_555
O5 O1 3.36(2) 1_555
O5 O1 2.61(2) 2_555
O5 O1 3.117(17) 6_556
O5 O3 2.840(19) 1_555
O5 O3 2.738(17) 2_555
O5 O3 2.628(17) 6_555
O5 O4 2.580(20) 2_555
O5 O5 3.013(13) 2_555
O5 O5 3.01(2) 3_555
O5 O5 3.142(18) 5_556
O5 O5 3.142(15) 6_556

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Pr1 O3 117.4(8) 1_555 2_555
O3 Pr1 O3 117.4(6) 1_555 3_555
O3 Pr1 O3 180.0(7) 1_555 4_555
O3 Pr1 O3 62.6(6) 1_555 5_555
O3 Pr1 O3 62.6(6) 1_555 6_555
O3 Pr1 O5 65.2(6) 1_555 1_555
O3 Pr1 O5 120.2(6) 1_555 2_555
O3 Pr1 O5 62.5(5) 1_555 3_555
O3 Pr1 O5 114.8(6) 1_555 4_555
O3 Pr1 O5 59.8(5) 1_555 5_555
O3 Pr1 O5 117.5(7) 1_555 6_555
O3 Pr1 O3 117.4(9) 2_555 3_555
O3 Pr1 O3 62.6(6) 2_555 4_555
O3 Pr1 O3 180.0(11) 2_555 5_555
O3 Pr1 O3 62.6(6) 2_555 6_555
O3 Pr1 O5 62.5(6) 2_555 1_555
O3 Pr1 O5 65.2(6) 2_555 2_555
O3 Pr1 O5 120.2(9) 2_555 3_555
O3 Pr1 O5 117.5(9) 2_555 4_555
O3 Pr1 O5 114.8(8) 2_555 5_555
O3 Pr1 O5 59.8(6) 2_555 6_555
O3 Pr1 O3 62.6(6) 3_555 4_555
O3 Pr1 O3 62.6(6) 3_555 5_555
O3 Pr1 O3 180.0(9) 3_555 6_555
O3 Pr1 O5 120.2(7) 3_555 1_555
O3 Pr1 O5 62.5(6) 3_555 2_555
O3 Pr1 O5 65.2(5) 3_555 3_555
O3 Pr1 O5 59.8(5) 3_555 4_555
O3 Pr1 O5 117.5(7) 3_555 5_555
O3 Pr1 O5 114.8(8) 3_555 6_555
O3 Pr1 O3 117.4(8) 4_555 5_555
O3 Pr1 O3 117.4(6) 4_555 6_555
O3 Pr1 O5 114.8(6) 4_555 1_555
O3 Pr1 O5 59.8(5) 4_555 2_555
O3 Pr1 O5 117.5(7) 4_555 3_555
O3 Pr1 O5 65.2(6) 4_555 4_555
O3 Pr1 O5 120.2(6) 4_555 5_555
O3 Pr1 O5 62.5(5) 4_555 6_555
O3 Pr1 O3 117.4(9) 5_555 6_555
O3 Pr1 O5 117.5(9) 5_555 1_555
O3 Pr1 O5 114.8(8) 5_555 2_555
O3 Pr1 O5 59.8(6) 5_555 3_555
O3 Pr1 O5 62.5(6) 5_555 4_555
O3 Pr1 O5 65.2(6) 5_555 5_555
O3 Pr1 O5 120.2(9) 5_555 6_555
O3 Pr1 O5 59.8(5) 6_555 1_555
O3 Pr1 O5 117.5(7) 6_555 2_555
O3 Pr1 O5 114.8(8) 6_555 3_555
O3 Pr1 O5 120.2(7) 6_555 4_555
O3 Pr1 O5 62.5(6) 6_555 5_555
O3 Pr1 O5 65.2(5) 6_555 6_555
O5 Pr1 O5 67.1(4) 1_555 2_555
O5 Pr1 O5 67.1(6) 1_555 3_555
O5 Pr1 O5 180.0(7) 1_555 4_555
O5 Pr1 O5 112.9(7) 1_555 5_555
O5 Pr1 O5 112.9(6) 1_555 6_555
O5 Pr1 O5 67.1(6) 2_555 3_555
O5 Pr1 O5 112.9(7) 2_555 4_555
O5 Pr1 O5 180.0(7) 2_555 5_555
O5 Pr1 O5 112.9(6) 2_555 6_555
O5 Pr1 O5 112.9(6) 3_555 4_555
O5 Pr1 O5 112.9(6) 3_555 5_555
O5 Pr1 O5 180.0(9) 3_555 6_555
O5 Pr1 O5 67.1(4) 4_555 5_555
O5 Pr1 O5 67.1(6) 4_555 6_555
O5 Pr1 O5 67.1(6) 5_555 6_555
O1 Pr2 O1 117.3(9) 2_655 4_656
O1 Pr2 O2 102.0(8) 2_655 4_655
O1 Pr2 O2 73.9(8) 2_655 11_555
O1 Pr2 O3 51.9(6) 2_655 2_655
O1 Pr2 O3 100.7(8) 2_655 4_655
O1 Pr2 O4 149.7(10) 2_655 3_655
O1 Pr2 O4 70.8(6) 2_655 4_656
O1 Pr2 O4 151.2(9) 2_655 18_545
O1 Pr2 O5 93.6(10) 2_655 2_655
O1 Pr2 O5 67.7(6) 2_655 6_656
O1 Pr2 O2 140.4(9) 4_656 4_655
O1 Pr2 O2 120.9(11) 4_656 11_555
O1 Pr2 O3 137.9(8) 4_656 2_655
O1 Pr2 O3 110.9(7) 4_656 4_655
O1 Pr2 O4 63.3(6) 4_656 3_655
O1 Pr2 O4 62.7(6) 4_656 4_656
O1 Pr2 O4 72.8(7) 4_656 18_545
O1 Pr2 O5 71.3(7) 4_656 2_655
O1 Pr2 O5 50.4(4) 4_656 6_656
O2 Pr2 O2 72.7(8) 4_655 11_555
O2 Pr2 O3 65.0(5) 4_655 2_655
O2 Pr2 O3 53.8(6) 4_655 4_655
O2 Pr2 O4 80.8(7) 4_655 3_655
O2 Pr2 O4 142.2(8) 4_655 4_656
O2 Pr2 O4 74.9(6) 4_655 18_545
O2 Pr2 O5 103.3(9) 4_655 2_655
O2 Pr2 O5 163.1(8) 4_655 6_656
O2 Pr2 O3 96.5(9) 11_555 2_655
O2 Pr2 O3 124.2(10) 11_555 4_655
O2 Pr2 O4 134.0(11) 11_555 3_655
O2 Pr2 O4 69.7(7) 11_555 4_656
O2 Pr2 O4 77.9(8) 11_555 18_545
O2 Pr2 O5 165.4(13) 11_555 2_655
O2 Pr2 O5 115.0(9) 11_555 6_656
O3 Pr2 O3 49.8(5) 2_655 4_655
O3 Pr2 O4 105.5(7) 2_655 3_655
O3 Pr2 O4 122.4(8) 2_655 4_656
O3 Pr2 O4 139.1(8) 2_655 18_545
O3 Pr2 O5 69.5(7) 2_655 2_655
O3 Pr2 O5 98.5(6) 2_655 6_656
O3 Pr2 O4 56.3(5) 4_655 3_655
O3 Pr2 O4 162.1(8) 4_655 4_656
O3 Pr2 O4 100.0(7) 4_655 18_545
O3 Pr2 O5 49.6(5) 4_655 2_655
O3 Pr2 O5 113.3(6) 4_655 6_656
O4 Pr2 O4 124.6(8) 3_655 4_656
O4 Pr2 O4 59.0(7) 3_655 18_545
O4 Pr2 O5 56.8(6) 3_655 2_655
O4 Pr2 O5 101.3(6) 3_655 6_656
O4 Pr2 O4 93.9(6) 4_656 18_545
O4 Pr2 O5 114.0(9) 4_656 2_655
O4 Pr2 O5 49.2(5) 4_656 6_656
O4 Pr2 O5 115.1(9) 18_545 2_655
O4 Pr2 O5 120.8(7) 18_545 6_656
O5 Pr2 O5 65.3(5) 2_655 6_656
O5 Zn1 O5 87.6(6) 1_555 2_555
O5 Zn1 O5 87.6(9) 1_555 3_555
O5 Zn1 O5 180.0(9) 1_555 4_556
O5 Zn1 O5 92.4(8) 1_555 5_556
O5 Zn1 O5 92.4(7) 1_555 6_556
O5 Zn1 O5 87.6(8) 2_555 3_555
O5 Zn1 O5 92.4(8) 2_555 4_556
O5 Zn1 O5 180.0(9) 2_555 5_556
O5 Zn1 O5 92.4(8) 2_555 6_556
O5 Zn1 O5 92.4(7) 3_555 4_556
O5 Zn1 O5 92.4(8) 3_555 5_556
O5 Zn1 O5 180.0(12) 3_555 6_556
O5 Zn1 O5 87.6(6) 4_556 5_556
O5 Zn1 O5 87.6(9) 4_556 6_556
O5 Zn1 O5 87.6(8) 5_556 6_556
O5 W1 O5 87.6(6) 1_555 2_555
O5 W1 O5 87.6(9) 1_555 3_555
O5 W1 O5 180.0(9) 1_555 4_556
O5 W1 O5 92.4(8) 1_555 5_556
O5 W1 O5 92.4(7) 1_555 6_556
O5 W1 O5 87.6(8) 2_555 3_555
O5 W1 O5 92.4(8) 2_555 4_556
O5 W1 O5 180.0(9) 2_555 5_556
O5 W1 O5 92.4(8) 2_555 6_556
O5 W1 O5 92.4(7) 3_555 4_556
O5 W1 O5 92.4(8) 3_555 5_556
O5 W1 O5 180.0(12) 3_555 6_556
O5 W1 O5 87.6(6) 4_556 5_556
O5 W1 O5 87.6(9) 4_556 6_556
O5 W1 O5 87.6(8) 5_556 6_556
O1 W2 O2 101.4(13) 1_555 1_555
O1 W2 O3 65.2(9) 1_555 1_555
O1 W2 O3 143.8(12) 1_555 5_555
O1 W2 O4 113.4(14) 1_555 1_555
O1 W2 O5 88.4(8) 1_555 3_555
O2 W2 O3 97.4(12) 1_555 1_555
O2 W2 O3 91.6(9) 1_555 5_555
O2 W2 O4 89.8(10) 1_555 1_555
O2 W2 O5 170.1(12) 1_555 3_555
O3 W2 O3 79.8(8) 1_555 5_555
O3 W2 O4 172.8(15) 1_555 1_555
O3 W2 O5 87.1(8) 1_555 3_555
O3 W2 O4 100.2(11) 5_555 1_555
O3 W2 O5 80.5(8) 5_555 3_555
O4 W2 O5 85.8(12) 1_555 3_555
Pr2 O1 Pr2 118.0(6) 3_665 4_656
Pr2 O1 W2 135.0(7) 3_665 1_555
Pr2 O1 O2 135.0(11) 3_665 1_555
Pr2 O1 O2 58.3(7) 3_665 10_555
Pr2 O1 O3 73.9(9) 3_665 1_555
Pr2 O1 O4 160.5(10) 3_665 1_555
Pr2 O1 O4 67.6(7) 3_665 6_556
Pr2 O1 O4 114.4(9) 3_665 9_555
Pr2 O1 O5 47.4(7) 3_665 1_555
Pr2 O1 O5 106.4(7) 3_665 3_555
Pr2 O1 O5 73.4(7) 3_665 5_556
Pr2 O1 W2 91.9(6) 4_656 1_555
Pr2 O1 O2 107.0(7) 4_656 1_555
Pr2 O1 O2 116.7(7) 4_656 10_555
Pr2 O1 O3 143.3(9) 4_656 1_555
Pr2 O1 O4 60.3(6) 4_656 1_555
Pr2 O1 O4 59.1(5) 4_656 6_556
Pr2 O1 O4 47.2(5) 4_656 9_555
Pr2 O1 O5 103.2(6) 4_656 1_555
Pr2 O1 O5 72.4(5) 4_656 3_555
Pr2 O1 O5 48.9(5) 4_656 5_556
W2 O1 O2 138.4(9) 1_555 10_555
W2 O1 O3 63.0(9) 1_555 1_555
W2 O1 O4 151.0(9) 1_555 6_556
W2 O1 O4 110.6(8) 1_555 9_555
W2 O1 O5 95.8(8) 1_555 1_555
W2 O1 O5 48.7(6) 1_555 3_555
W2 O1 O5 112.2(8) 1_555 5_556
O2 O1 O2 100.7(9) 1_555 10_555
O2 O1 O3 71.1(10) 1_555 1_555
O2 O1 O4 52.1(7) 1_555 1_555
O2 O1 O4 144.0(10) 1_555 6_556
O2 O1 O4 94.4(8) 1_555 9_555
O2 O1 O5 124.8(10) 1_555 1_555
O2 O1 O5 87.9(8) 1_555 3_555
O2 O1 O5 147.7(9) 1_555 5_556
O2 O1 O3 99.3(9) 10_555 1_555
O2 O1 O4 141.1(10) 10_555 1_555
O2 O1 O4 65.0(6) 10_555 6_556
O2 O1 O4 75.4(8) 10_555 9_555
O2 O1 O5 105.4(7) 10_555 1_555
O2 O1 O5 164.3(8) 10_555 3_555
O2 O1 O5 109.4(7) 10_555 5_556
O3 O1 O4 96.6(11) 1_555 1_555
O3 O1 O4 141.1(10) 1_555 6_556
O3 O1 O4 163.6(11) 1_555 9_555
O3 O1 O5 57.4(8) 1_555 1_555
O3 O1 O5 70.8(8) 1_555 3_555
O3 O1 O5 113.8(9) 1_555 5_556
O4 O1 O4 118.2(9) 1_555 6_556
O4 O1 O4 79.4(7) 1_555 9_555
O4 O1 O5 113.1(9) 1_555 1_555
O4 O1 O5 54.1(7) 1_555 3_555
O4 O1 O5 96.0(8) 1_555 5_556
O4 O1 O4 50.9(7) 6_556 9_555
O4 O1 O5 91.2(7) 6_556 1_555
O4 O1 O5 114.8(7) 6_556 3_555
O4 O1 O5 49.8(5) 6_556 5_556
O4 O1 O5 138.8(9) 9_555 1_555
O4 O1 O5 117.4(8) 9_555 3_555
O4 O1 O5 82.5(7) 9_555 5_556
O5 O1 O5 59.1(6) 1_555 3_555
O5 O1 O5 57.9(6) 1_555 5_556
O5 O1 O5 65.9(6) 3_555 5_556
Pr2 O2 Pr2 109.5(4) 4_655 12_445
Pr2 O2 W2 100.1(5) 4_655 1_555
Pr2 O2 O1 119.8(8) 4_655 1_555
Pr2 O2 O1 102.8(6) 4_655 10_555
Pr2 O2 O2 159.1(7) 4_655 9_555
Pr2 O2 O2 49.9(6) 4_655 14_544
Pr2 O2 O3 76.8(7) 4_655 1_555
Pr2 O2 O3 54.5(5) 4_655 5_555
Pr2 O2 O4 119.0(7) 4_655 1_555
Pr2 O2 O4 48.6(5) 4_655 9_554
Pr2 O2 O4 97.8(8) 4_655 14_544
Pr2 O2 W2 149.1(5) 12_445 1_555
Pr2 O2 O1 113.9(8) 12_445 1_555
Pr2 O2 O1 47.8(6) 12_445 10_555
Pr2 O2 O2 57.4(6) 12_445 9_555
Pr2 O2 O2 84.3(6) 12_445 14_544
Pr2 O2 O3 134.1(8) 12_445 1_555
Pr2 O2 O3 161.8(6) 12_445 5_555
Pr2 O2 O4 120.5(7) 12_445 1_555
Pr2 O2 O4 63.0(5) 12_445 9_554
Pr2 O2 O4 50.7(6) 12_445 14_544
W2 O2 O1 117.5(8) 1_555 10_555
W2 O2 O2 96.5(8) 1_555 9_555
W2 O2 O2 123.0(9) 1_555 14_544
W2 O2 O3 49.0(6) 1_555 5_555
W2 O2 O4 46.0(7) 1_555 1_555
W2 O2 O4 140.8(8) 1_555 9_554
W2 O2 O4 134.7(11) 1_555 14_544
O1 O2 O1 79.3(8) 1_555 10_555
O1 O2 O2 81.1(9) 1_555 9_555
O1 O2 O2 161.8(11) 1_555 14_544
O1 O2 O3 83.6(8) 1_555 5_555
O1 O2 O4 69.4(9) 1_555 1_555
O1 O2 O4 128.3(9) 1_555 9_554
O1 O2 O4 142.1(12) 1_555 14_544
O1 O2 O2 80.5(8) 10_555 9_555
O1 O2 O2 116.1(9) 10_555 14_544
O1 O2 O3 86.4(8) 10_555 1_555
O1 O2 O3 137.8(7) 10_555 5_555
O1 O2 O4 136.2(9) 10_555 1_555
O1 O2 O4 61.6(6) 10_555 9_554
O1 O2 O4 98.3(10) 10_555 14_544
O2 O2 O2 109.9(8) 9_555 14_544
O2 O2 O3 124.1(10) 9_555 1_555
O2 O2 O3 134.4(8) 9_555 5_555
O2 O2 O4 65.5(7) 9_555 1_555
O2 O2 O4 120.3(8) 9_555 9_554
O2 O2 O4 61.3(7) 9_555 14_544
O2 O2 O3 124.5(10) 14_544 1_555
O2 O2 O3 78.3(7) 14_544 5_555
O2 O2 O4 101.4(8) 14_544 1_555
O2 O2 O4 59.4(7) 14_544 9_554
O2 O2 O4 49.4(7) 14_544 14_544
O3 O2 O3 55.9(7) 1_555 5_555
O3 O2 O4 90.6(9) 1_555 1_555
O3 O2 O4 99.1(8) 1_555 9_554
O3 O2 O4 173.6(12) 1_555 14_544
O3 O2 O4 68.9(7) 5_555 1_555
O3 O2 O4 102.8(7) 5_555 9_554
O3 O2 O4 118.2(9) 5_555 14_544
O4 O2 O4 160.7(8) 1_555 9_554
O4 O2 O4 89.0(9) 1_555 14_544
O4 O2 O4 79.6(8) 9_554 14_544
Pr1 O3 Pr2 115.4(4) 1_555 3_665
Pr1 O3 Pr2 89.7(3) 1_555 4_655
Pr1 O3 W2 96.3(5) 1_555 1_555
Pr1 O3 W2 94.0(4) 1_555 6_555
Pr1 O3 O1 124.3(8) 1_555 1_555
Pr1 O3 O2 119.4(8) 1_555 1_555
Pr1 O3 O2 121.7(6) 1_555 6_555
Pr1 O3 O3 58.7(6) 1_555 5_555
Pr1 O3 O3 58.7(6) 1_555 6_555
Pr1 O3 O4 116.9(6) 1_555 6_555
Pr1 O3 O5 60.6(5) 1_555 1_555
Pr1 O3 O5 62.0(5) 1_555 3_555
Pr1 O3 O5 63.6(5) 1_555 5_555
Pr2 O3 Pr2 154.7(4) 3_665 4_655
Pr2 O3 W2 105.1(5) 3_665 1_555
Pr2 O3 W2 96.9(5) 3_665 6_555
Pr2 O3 O1 54.2(8) 3_665 1_555
Pr2 O3 O2 114.3(9) 3_665 1_555
Pr2 O3 O2 60.5(6) 3_665 6_555
Pr2 O3 O3 150.5(8) 3_665 5_555
Pr2 O3 O3 83.7(7) 3_665 6_555
Pr2 O3 O4 108.5(6) 3_665 6_555
Pr2 O3 O5 54.9(5) 3_665 1_555
Pr2 O3 O5 92.6(6) 3_665 3_555
Pr2 O3 O5 141.6(7) 3_665 5_555
Pr2 O3 W2 73.7(5) 4_655 1_555
Pr2 O3 W2 76.9(5) 4_655 6_555
Pr2 O3 O1 115.3(8) 4_655 1_555
Pr2 O3 O2 49.4(6) 4_655 1_555
Pr2 O3 O2 104.3(7) 4_655 6_555
Pr2 O3 O3 46.4(5) 4_655 5_555
Pr2 O3 O3 108.4(7) 4_655 6_555
Pr2 O3 O4 52.7(5) 4_655 6_555
Pr2 O3 O5 150.3(7) 4_655 1_555
Pr2 O3 O5 102.9(5) 4_655 3_555
Pr2 O3 O5 45.9(5) 4_655 5_555
W2 O3 W2 148.7(6) 1_555 6_555
W2 O3 O1 51.9(8) 1_555 1_555
W2 O3 O2 142.0(10) 1_555 6_555
W2 O3 O3 51.6(6) 1_555 5_555
W2 O3 O3 154.5(10) 1_555 6_555
W2 O3 O4 113.7(7) 1_555 6_555
W2 O3 O5 108.1(8) 1_555 1_555
W2 O3 O5 45.6(6) 1_555 3_555
W2 O3 O5 113.2(8) 1_555 5_555
W2 O3 O1 138.2(10) 6_555 1_555
W2 O3 O2 112.1(9) 6_555 1_555
W2 O3 O3 112.0(8) 6_555 5_555
W2 O3 O3 48.6(7) 6_555 6_555
W2 O3 O5 102.7(7) 6_555 1_555
W2 O3 O5 156.0(7) 6_555 3_555
W2 O3 O5 47.4(6) 6_555 5_555
O1 O3 O2 65.9(10) 1_555 1_555
O1 O3 O2 100.2(11) 1_555 6_555
O1 O3 O3 103.0(10) 1_555 5_555
O1 O3 O3 136.0(12) 1_555 6_555
O1 O3 O4 117.7(10) 1_555 6_555
O1 O3 O5 85.2(10) 1_555 1_555
O1 O3 O5 64.2(7) 1_555 3_555
O1 O3 O5 161.2(11) 1_555 5_555
O2 O3 O2 111.8(11) 1_555 6_555
O2 O3 O3 60.9(7) 1_555 5_555
O2 O3 O3 156.9(12) 1_555 6_555
O2 O3 O4 75.9(8) 1_555 6_555
O2 O3 O5 144.8(11) 1_555 1_555
O2 O3 O5 83.4(8) 1_555 3_555
O2 O3 O5 95.3(9) 1_555 5_555
O2 O3 O3 148.8(10) 6_555 5_555
O2 O3 O3 63.2(7) 6_555 6_555
O2 O3 O4 51.7(6) 6_555 6_555
O2 O3 O5 92.0(7) 6_555 1_555
O2 O3 O5 152.5(9) 6_555 3_555
O2 O3 O5 86.6(7) 6_555 5_555
O3 O3 O3 110.6(10) 5_555 6_555
O3 O3 O4 98.6(7) 5_555 6_555
O3 O3 O5 110.4(9) 5_555 1_555
O3 O3 O5 58.5(6) 5_555 3_555
O3 O3 O5 65.2(7) 5_555 5_555
O3 O3 O4 84.9(8) 6_555 6_555
O3 O3 O5 57.2(7) 6_555 1_555
O3 O3 O5 111.2(9) 6_555 3_555
O3 O3 O5 62.6(8) 6_555 5_555
O4 O3 O5 138.1(8) 6_555 1_555
O4 O3 O5 155.0(7) 6_555 3_555
O4 O3 O5 53.8(6) 6_555 5_555
O5 O3 O5 65.4(7) 1_555 3_555
O5 O3 O5 112.2(8) 1_555 5_555
O5 O3 O5 115.6(8) 3_555 5_555
Pr2 O4 Pr2 94.0(3) 2_545 4_656
Pr2 O4 Pr2 121.0(5) 2_545 17_555
Pr2 O4 W2 96.8(6) 2_545 1_555
Pr2 O4 O1 108.2(6) 2_545 1_555
Pr2 O4 O1 57.6(5) 2_545 5_556
Pr2 O4 O1 89.3(6) 2_545 14_544
Pr2 O4 O2 130.4(6) 2_545 1_555
Pr2 O4 O2 164.3(6) 2_545 9_555
Pr2 O4 O2 105.1(6) 2_545 14_545
Pr2 O4 O3 71.0(5) 2_545 5_555
Pr2 O4 O4 51.4(6) 2_545 16_545
Pr2 O4 O5 53.6(6) 2_545 3_555
Pr2 O4 Pr2 102.0(5) 4_656 17_555
Pr2 O4 W2 87.7(6) 4_656 1_555
Pr2 O4 O1 57.0(6) 4_656 1_555
Pr2 O4 O1 160.1(8) 4_656 14_544
Pr2 O4 O2 109.8(7) 4_656 1_555
Pr2 O4 O2 76.2(5) 4_656 9_555
Pr2 O4 O2 47.3(5) 4_656 14_545
Pr2 O4 O3 122.8(6) 4_656 5_555
Pr2 O4 O4 105.3(7) 4_656 16_545
Pr2 O4 O5 71.1(7) 4_656 3_555
Pr2 O4 W2 139.7(7) 17_555 1_555
Pr2 O4 O1 128.2(10) 17_555 1_555
Pr2 O4 O1 102.4(8) 17_555 5_556
Pr2 O4 O1 60.0(7) 17_555 14_544
Pr2 O4 O2 96.5(8) 17_555 1_555
Pr2 O4 O2 51.4(6) 17_555 9_555
Pr2 O4 O2 56.5(6) 17_555 14_545
Pr2 O4 O3 133.6(8) 17_555 5_555
Pr2 O4 O4 69.6(7) 17_555 16_545
Pr2 O4 O5 169.7(10) 17_555 3_555
W2 O4 O1 110.0(8) 1_555 5_556
W2 O4 O1 111.5(10) 1_555 14_544
W2 O4 O2 94.9(8) 1_555 9_555
W2 O4 O2 130.2(10) 1_555 14_545
W2 O4 O4 145.5(10) 1_555 16_545
W2 O4 O5 49.3(8) 1_555 3_555
O1 O4 O1 89.9(8) 1_555 5_556
O1 O4 O1 139.8(11) 1_555 14_544
O1 O4 O2 58.6(8) 1_555 1_555
O1 O4 O2 76.9(8) 1_555 9_555
O1 O4 O2 97.4(9) 1_555 14_545
O1 O4 O3 75.4(7) 1_555 5_555
O1 O4 O4 154.8(11) 1_555 16_545
O1 O4 O5 55.0(7) 1_555 3_555
O1 O4 O1 129.1(9) 5_556 14_544
O1 O4 O2 148.4(9) 5_556 1_555
O1 O4 O2 108.4(7) 5_556 9_555
O1 O4 O2 53.4(6) 5_556 14_545
O1 O4 O3 118.5(8) 5_556 5_555
O1 O4 O4 67.1(7) 5_556 16_545
O1 O4 O5 67.3(8) 5_556 3_555
O1 O4 O2 82.4(8) 14_544 1_555
O1 O4 O2 96.0(7) 14_544 9_555
O1 O4 O2 112.9(8) 14_544 14_545
O1 O4 O3 76.8(8) 14_544 5_555
O1 O4 O4 62.0(7) 14_544 16_545
O1 O4 O5 125.3(11) 14_544 3_555
O2 O4 O2 65.1(7) 1_555 9_555
O2 O4 O2 123.2(9) 1_555 14_545
O2 O4 O3 59.4(6) 1_555 5_555
O2 O4 O4 144.2(10) 1_555 16_545
O2 O4 O5 93.1(9) 1_555 3_555
O2 O4 O2 59.2(6) 9_555 14_545
O2 O4 O3 124.6(8) 9_555 5_555
O2 O4 O4 119.0(7) 9_555 16_545
O2 O4 O5 131.1(10) 9_555 3_555
O2 O4 O3 169.8(9) 14_545 5_555
O2 O4 O4 77.5(7) 14_545 16_545
O2 O4 O5 114.7(10) 14_545 3_555
O3 O4 O4 105.8(9) 5_555 16_545
O3 O4 O5 55.3(7) 5_555 3_555
O4 O4 O5 104.3(10) 16_545 3_555
Pr1 O5 Pr2 109.9(3) 1_555 3_665
Pr1 O5 Pr2 154.1(3) 1_555 5_566
Pr1 O5 Zn1 87.3(4) 1_555 1_555
Pr1 O5 W1 87.3(4) 1_555 1_555
Pr1 O5 W2 91.9(5) 1_555 2_555
Pr1 O5 O1 83.2(5) 1_555 1_555
Pr1 O5 O1 99.3(8) 1_555 2_555
Pr1 O5 O1 164.4(7) 1_555 6_556
Pr1 O5 O3 54.3(5) 1_555 1_555
Pr1 O5 O3 55.4(5) 1_555 2_555
Pr1 O5 O3 56.6(5) 1_555 6_555
Pr1 O5 O4 126.9(7) 1_555 2_555
Pr1 O5 O5 56.4(4) 1_555 2_555
Pr1 O5 O5 56.4(5) 1_555 3_555
Pr1 O5 O5 117.7(5) 1_555 5_556
Pr1 O5 O5 117.7(5) 1_555 6_556
Pr2 O5 Pr2 95.9(3) 3_665 5_566
Pr2 O5 Zn1 108.5(4) 3_665 1_555
Pr2 O5 W1 108.5(4) 3_665 1_555
Pr2 O5 W2 107.7(5) 3_665 2_555
Pr2 O5 O1 139.9(8) 3_665 2_555
Pr2 O5 O1 59.8(5) 3_665 6_556
Pr2 O5 O3 55.7(5) 3_665 1_555
Pr2 O5 O3 143.1(6) 3_665 2_555
Pr2 O5 O3 84.4(6) 3_665 6_555
Pr2 O5 O4 69.6(7) 3_665 2_555
Pr2 O5 O5 146.6(5) 3_665 2_555
Pr2 O5 O5 86.8(6) 3_665 3_555
Pr2 O5 O5 68.9(5) 3_665 5_556
Pr2 O5 O5 119.6(5) 3_665 6_556
Pr2 O5 Zn1 86.6(4) 5_566 1_555
Pr2 O5 W1 86.6(4) 5_566 1_555
Pr2 O5 W2 77.7(5) 5_566 2_555
Pr2 O5 O1 120.3(7) 5_566 1_555
Pr2 O5 O1 57.2(6) 5_566 2_555
Pr2 O5 O3 151.5(7) 5_566 1_555
Pr2 O5 O3 102.2(6) 5_566 2_555
Pr2 O5 O3 126.5(7) 5_566 6_555
Pr2 O5 O4 59.7(5) 5_566 2_555
Pr2 O5 O5 102.6(5) 5_566 2_555
Pr2 O5 O5 129.9(7) 5_566 3_555
Pr2 O5 O5 73.1(5) 5_566 5_556
Pr2 O5 O5 45.8(4) 5_566 6_556
Zn1 O5 W2 141.7(5) 1_555 2_555
Zn1 O5 O1 79.7(6) 1_555 1_555
Zn1 O5 O1 99.5(9) 1_555 2_555
Zn1 O5 O1 85.6(6) 1_555 6_556
Zn1 O5 O3 101.3(7) 1_555 1_555
Zn1 O5 O3 104.5(7) 1_555 2_555
Zn1 O5 O3 143.8(8) 1_555 6_555
Zn1 O5 O4 145.1(9) 1_555 2_555
Zn1 O5 O5 46.2(4) 1_555 2_555
Zn1 O5 O5 46.2(6) 1_555 3_555
W1 O5 W2 141.7(5) 1_555 2_555
W1 O5 O1 79.7(6) 1_555 1_555
W1 O5 O1 99.5(9) 1_555 2_555
W1 O5 O1 85.6(6) 1_555 6_556
W1 O5 O3 101.3(7) 1_555 1_555
W1 O5 O3 104.5(7) 1_555 2_555
W1 O5 O3 143.8(8) 1_555 6_555
W1 O5 O4 145.1(9) 1_555 2_555
W1 O5 O5 46.2(4) 1_555 2_555
W1 O5 O5 46.2(6) 1_555 3_555
W2 O5 O1 138.2(9) 2_555 1_555
W2 O5 O1 102.2(7) 2_555 6_556
W2 O5 O3 109.1(8) 2_555 1_555
W2 O5 O3 47.2(6) 2_555 2_555
W2 O5 O3 52.1(7) 2_555 6_555
W2 O5 O5 103.4(6) 2_555 2_555
W2 O5 O5 148.3(9) 2_555 3_555
W2 O5 O5 150.0(8) 2_555 5_556
W2 O5 O5 105.8(7) 2_555 6_556
O1 O5 O1 177.4(11) 1_555 2_555
O1 O5 O1 82.0(7) 1_555 6_556
O1 O5 O3 137.6(9) 1_555 2_555
O1 O5 O3 92.5(8) 1_555 6_555
O1 O5 O4 108.2(10) 1_555 2_555
O1 O5 O5 107.9(6) 1_555 2_555
O1 O5 O5 47.9(6) 1_555 3_555
O1 O5 O5 57.2(6) 1_555 5_556
O1 O5 O5 113.3(7) 1_555 6_556
O1 O5 O1 95.5(8) 2_555 6_556
O1 O5 O3 145.0(11) 2_555 1_555
O1 O5 O3 89.6(8) 2_555 6_555
O1 O5 O4 71.0(8) 2_555 2_555
O1 O5 O5 73.0(8) 2_555 2_555
O1 O5 O5 133.0(11) 2_555 3_555
O1 O5 O5 120.6(10) 2_555 5_556
O1 O5 O5 64.9(7) 2_555 6_556
O1 O5 O3 113.8(8) 6_556 1_555
O1 O5 O3 140.0(8) 6_556 2_555
O1 O5 O3 128.6(8) 6_556 6_555
O1 O5 O4 62.9(7) 6_556 2_555
O1 O5 O5 124.8(6) 6_556 2_555
O1 O5 O5 109.4(8) 6_556 3_555
O1 O5 O5 49.3(6) 6_556 5_556
O1 O5 O5 64.9(5) 6_556 6_556
O3 O5 O3 102.2(8) 1_555 2_555
O3 O5 O3 57.6(7) 1_555 6_555
O3 O5 O4 104.9(10) 1_555 2_555
O3 O5 O5 102.5(6) 1_555 2_555
O3 O5 O5 55.7(6) 1_555 3_555
O3 O5 O5 93.6(7) 1_555 5_556
O3 O5 O5 144.3(8) 1_555 6_556
O3 O5 O3 58.9(6) 2_555 6_555
O3 O5 O4 92.1(7) 2_555 2_555
O3 O5 O5 58.9(6) 2_555 2_555
O3 O5 O5 105.0(9) 2_555 3_555
O3 O5 O5 147.4(8) 2_555 5_556
O3 O5 O5 95.7(7) 2_555 6_556
O3 O5 O4 70.9(8) 6_555 2_555
O3 O5 O5 105.7(7) 6_555 2_555
O3 O5 O5 103.5(8) 6_555 3_555
O3 O5 O5 149.3(9) 6_555 5_556
O3 O5 O5 153.4(8) 6_555 6_556
O4 O5 O5 143.8(8) 2_555 2_555
O4 O5 O5 156.0(11) 2_555 3_555
O4 O5 O5 111.3(9) 2_555 5_556
O4 O5 O5 105.1(7) 2_555 6_556
O5 O5 O5 60.0(6) 2_555 3_555
O5 O5 O5 90.0(6) 2_555 5_556
O5 O5 O5 61.3(5) 2_555 6_556
O5 O5 O5 61.3(6) 3_555 5_556
O5 O5 O5 90.0(7) 3_555 6_556
O5 O5 O5 57.3(5) 5_556 6_556

#=============================================================================

# STRUCTURE FACTORS :

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Pr700W625Co75O3000
_database_code_depnum_ccdc_archive 'CCDC 1894710'
loop_
_audit_author_name
_audit_author_address
'Philippe Lacorre' 'IMMM, UMR 6283 CNRS, Le Mans Universit?, France'
_audit_update_record             
;
2019-01-30 deposited with the CCDC.	2019-03-13 downloaded from the CCDC.
;

_pd_block_id                     Pr7W6.25Co0.75O30

#=============================================================================

# POWDER DIFFRACTOMETER CHARACTERISTICS : 

_diffrn_measurement_device_type  'PANalytical Empyrean'
_diffrn_radiation_type           'X-ray Cu K\a'
loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
1.54056 1.0000
1.54439 0.5000

_pd_spec_mount_mode              reflection
_pd_meas_scan_method             step

_diffrn_ambient_temperature      300

#=============================================================================

# COMPOUND FORMULATION & CHARACTERISTICS : 

# Formula

_chemical_formula_moiety         'Co0.75 O30 Pr7 W6.25'
_chemical_formula_sum            'Co0.75 O30 Pr7 W6.25'
_chemical_formula_weight         2659.52

# Colour

_pd_char_colour                  'light olive green'


# Density

_exptl_crystal_density_diffrn    7.930

# Symmetry

_symmetry_cell_setting           Trigonal
_symmetry_space_group_name_H-M   'R -3'
_symmetry_space_group_name_Hall  '-R 3'

loop_
_symmetry_equiv_pos_as_xyz
x,y,z
-y,x-y,z
-x+y,-x,z
-x,-y,-z
y,-x+y,-z
x-y,x,-z
x+2/3,y+1/3,z+1/3
-y+2/3,x-y+1/3,z+1/3
-x+y+2/3,-x+1/3,z+1/3
-x+2/3,-y+1/3,-z+1/3
y+2/3,-x+y+1/3,-z+1/3
x-y+2/3,x+1/3,-z+1/3
x+1/3,y+2/3,z+2/3
-y+1/3,x-y+2/3,z+2/3
-x+y+1/3,-x+2/3,z+2/3
-x+1/3,-y+2/3,-z+2/3
y+1/3,-x+y+2/3,-z+2/3
x-y+1/3,x+2/3,-z+2/3

# Cell parameters

_cell_length_a                   16.8341(2)
_cell_length_b                   16.8341(2)
_cell_length_c                   6.8079(1)
_cell_angle_alpha                90.0000
_cell_angle_beta                 90.0000
_cell_angle_gamma                120.000
_cell_volume                     1670.79(3)
_cell_formula_units_Z            3
_cell_measurement_temperature    300

#=============================================================================

# REFINEMENT DATA :

#  Data used in refinement :

_pd_proc_2theta_range_min        9.000
_pd_proc_2theta_range_max        130.000
_pd_proc_2theta_range_inc        0.0131


#  Refinement program and convergence

_computing_structure_refinement  FULLPROF
_refine_ls_shift/su_max          0.01


#  Reliability factors for points with Bragg contributions

_pd_proc_ls_prof_R_factor        6.65
_pd_proc_ls_prof_wR_factor       6.99
_pd_proc_ls_prof_wR_expected     2.36

_refine_ls_R_I_factor            4.18
_refine_ls_goodness_of_fit_all   3.06

#=============================================================================

# ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS :

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_Wyckoff_symbol
_atom_site_thermal_displace_type
_atom_site_B_iso_or_equiv
Pr1 Pr+3 0.0000 0.0000 0.0000 1.000 3 a Biso 0.94(5)
Pr2 Pr+3 0.7799(1) -0.0134(2) 0.3346(5) 1.000 18 f Biso 0.94(5)
Co1 Co+2 0.0000 0.0000 0.5000 0.750 3 b Biso 0.43(3)
W1 W+6 0.0000 0.0000 0.5000 0.250 3 b Biso 0.43(3)
W2 W+6 0.1964(1) 0.0127(1) 0.1705(4) 1.000 18 f Biso 0.43(3)
O1 O-2 0.241(1) 0.097(2) 0.347(4) 1.000 18 f Biso 2.2(2)
O2 O-2 0.293(2) 0.044(2) 0.005(4) 1.000 18 f Biso 2.2(2)
O3 O-2 0.172(1) 0.114(2) 0.055(4) 1.000 18 f Biso 2.2(2)
O4 O-2 0.209(2) -0.075(2) 0.301(3) 1.000 18 f Biso 2.2(2)
O5 O-2 0.039(1) 0.114(1) 0.318(3) 1.000 18 f Biso 2.1(2)

_chemical_formula_structural     'Pr Pr6 (Co0.75W0.25) W6 (O6)5'

#=============================================================================

# DISTANCES AND ANGLES :

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pr1 O3 2.577(5) 1_555
Pr1 O3 2.577(9) 2_555
Pr1 O3 2.577(8) 3_555
Pr1 O3 2.577(5) 4_555
Pr1 O3 2.577(9) 5_555
Pr1 O3 2.577(8) 6_555
Pr1 O5 2.748(7) 1_555
Pr1 O5 2.748(7) 2_555
Pr1 O5 2.748(8) 3_555
Pr1 O5 2.748(7) 4_555
Pr1 O5 2.748(7) 5_555
Pr1 O5 2.748(8) 6_555
Pr2 O1 2.417(7) 2_655
Pr2 O1 2.511(9) 4_656
Pr2 O2 2.545(8) 4_655
Pr2 O2 2.452(12) 11_555
Pr2 O3 2.479(7) 2_655
Pr2 O3 3.448(9) 4_655
Pr2 O4 2.915(8) 3_655
Pr2 O4 2.852(7) 4_656
Pr2 O4 2.428(7) 18_545
Pr2 O5 2.481(10) 2_655
Pr2 O5 3.187(7) 6_656
Co1 O5 2.095(7) 1_555
Co1 O5 2.095(7) 2_555
Co1 O5 2.095(9) 3_555
Co1 O5 2.095(7) 4_556
Co1 O5 2.095(7) 5_556
Co1 O5 2.095(9) 6_556
W1 O5 2.095(7) 1_555
W1 O5 2.095(7) 2_555
W1 O5 2.095(9) 3_555
W1 O5 2.095(7) 4_556
W1 O5 2.095(7) 5_556
W1 O5 2.095(9) 6_556
W2 O1 1.720(8) 1_555
W2 O2 1.820(8) 1_555
W2 O3 2.090(9) 1_555
W2 O3 2.015(7) 5_555
W2 O4 1.829(9) 1_555
W2 O5 2.038(7) 3_555
O1 O2 2.782(13) 1_555
O1 O2 2.874(11) 10_555
O1 O3 2.392(12) 1_555
O1 O4 2.690(13) 1_555
O1 O4 2.906(11) 6_556
O1 O4 2.931(11) 9_555
O1 O5 2.584(8) 3_555
O1 O5 3.021(11) 5_556
O2 O1 2.782(13) 1_555
O2 O1 2.874(11) 10_555
O2 O2 3.119(13) 9_555
O2 O2 3.119(13) 14_544
O2 O3 2.825(14) 1_555
O2 O3 2.652(9) 5_555
O2 O4 2.693(10) 1_555
O2 O4 2.905(10) 9_554
O2 O4 3.066(15) 14_544
O3 O1 2.392(12) 1_555
O3 O2 2.825(14) 1_555
O3 O2 2.652(12) 6_555
O3 O3 2.656(11) 5_555
O3 O3 2.656(13) 6_555
O3 O4 2.997(10) 6_555
O3 O5 2.876(12) 1_555
O3 O5 2.874(9) 3_555
O3 O5 2.680(10) 5_555
O4 O1 2.690(13) 1_555
O4 O1 2.906(10) 5_556
O4 O1 2.931(13) 14_544
O4 O2 2.693(10) 1_555
O4 O2 3.066(10) 9_555
O4 O2 2.905(12) 14_545
O4 O3 2.997(11) 5_555
O4 O4 2.699(11) 16_545
O4 O5 2.616(14) 3_555
O5 O1 2.584(13) 2_555
O5 O1 3.021(10) 6_556
O5 O3 2.876(12) 1_555
O5 O3 2.874(10) 2_555
O5 O3 2.680(11) 6_555
O5 O4 2.616(11) 2_555
O5 O5 2.928(7) 2_555
O5 O5 2.928(12) 3_555
O5 O5 2.997(11) 5_556
O5 O5 2.997(9) 6_556

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Pr1 O3 117.9(5) 1_555 2_555
O3 Pr1 O3 117.9(4) 1_555 3_555
O3 Pr1 O3 180.0(4) 1_555 4_555
O3 Pr1 O3 62.1(3) 1_555 5_555
O3 Pr1 O3 62.1(4) 1_555 6_555
O3 Pr1 O5 65.3(3) 1_555 1_555
O3 Pr1 O5 119.7(4) 1_555 2_555
O3 Pr1 O5 65.2(3) 1_555 3_555
O3 Pr1 O5 114.7(4) 1_555 4_555
O3 Pr1 O5 60.3(3) 1_555 5_555
O3 Pr1 O5 114.8(4) 1_555 6_555
O3 Pr1 O3 117.9(6) 2_555 3_555
O3 Pr1 O3 62.1(3) 2_555 4_555
O3 Pr1 O3 180.0(6) 2_555 5_555
O3 Pr1 O3 62.1(3) 2_555 6_555
O3 Pr1 O5 65.2(3) 2_555 1_555
O3 Pr1 O5 65.3(4) 2_555 2_555
O3 Pr1 O5 119.7(5) 2_555 3_555
O3 Pr1 O5 114.8(5) 2_555 4_555
O3 Pr1 O5 114.7(5) 2_555 5_555
O3 Pr1 O5 60.3(4) 2_555 6_555
O3 Pr1 O3 62.1(4) 3_555 4_555
O3 Pr1 O3 62.1(3) 3_555 5_555
O3 Pr1 O3 180.0(6) 3_555 6_555
O3 Pr1 O5 119.7(4) 3_555 1_555
O3 Pr1 O5 65.2(4) 3_555 2_555
O3 Pr1 O5 65.3(3) 3_555 3_555
O3 Pr1 O5 60.3(3) 3_555 4_555
O3 Pr1 O5 114.8(4) 3_555 5_555
O3 Pr1 O5 114.7(5) 3_555 6_555
O3 Pr1 O3 117.9(5) 4_555 5_555
O3 Pr1 O3 117.9(4) 4_555 6_555
O3 Pr1 O5 114.7(4) 4_555 1_555
O3 Pr1 O5 60.3(3) 4_555 2_555
O3 Pr1 O5 114.8(4) 4_555 3_555
O3 Pr1 O5 65.3(3) 4_555 4_555
O3 Pr1 O5 119.7(4) 4_555 5_555
O3 Pr1 O5 65.2(3) 4_555 6_555
O3 Pr1 O3 117.9(6) 5_555 6_555
O3 Pr1 O5 114.8(5) 5_555 1_555
O3 Pr1 O5 114.7(5) 5_555 2_555
O3 Pr1 O5 60.3(4) 5_555 3_555
O3 Pr1 O5 65.2(3) 5_555 4_555
O3 Pr1 O5 65.3(4) 5_555 5_555
O3 Pr1 O5 119.7(5) 5_555 6_555
O3 Pr1 O5 60.3(3) 6_555 1_555
O3 Pr1 O5 114.8(4) 6_555 2_555
O3 Pr1 O5 114.7(5) 6_555 3_555
O3 Pr1 O5 119.7(4) 6_555 4_555
O3 Pr1 O5 65.2(4) 6_555 5_555
O3 Pr1 O5 65.3(3) 6_555 6_555
O5 Pr1 O5 64.4(3) 1_555 2_555
O5 Pr1 O5 64.4(3) 1_555 3_555
O5 Pr1 O5 180.0(4) 1_555 4_555
O5 Pr1 O5 115.6(4) 1_555 5_555
O5 Pr1 O5 115.6(4) 1_555 6_555
O5 Pr1 O5 64.4(3) 2_555 3_555
O5 Pr1 O5 115.6(4) 2_555 4_555
O5 Pr1 O5 180.0(4) 2_555 5_555
O5 Pr1 O5 115.6(4) 2_555 6_555
O5 Pr1 O5 115.6(4) 3_555 4_555
O5 Pr1 O5 115.6(4) 3_555 5_555
O5 Pr1 O5 180.0(5) 3_555 6_555
O5 Pr1 O5 64.4(3) 4_555 5_555
O5 Pr1 O5 64.4(3) 4_555 6_555
O5 Pr1 O5 64.4(3) 5_555 6_555
O1 Pr2 O1 112.9(5) 2_655 4_656
O1 Pr2 O2 108.4(4) 2_655 4_655
O1 Pr2 O2 72.4(4) 2_655 11_555
O1 Pr2 O3 58.5(4) 2_655 2_655
O1 Pr2 O3 106.3(5) 2_655 4_655
O1 Pr2 O4 150.7(5) 2_655 3_655
O1 Pr2 O4 66.3(3) 2_655 4_656
O1 Pr2 O4 149.3(4) 2_655 18_545
O1 Pr2 O5 93.5(5) 2_655 2_655
O1 Pr2 O5 63.5(3) 2_655 6_656
O1 Pr2 O2 138.7(6) 4_656 4_655
O1 Pr2 O2 114.3(7) 4_656 11_555
O1 Pr2 O3 143.3(5) 4_656 2_655
O1 Pr2 O3 113.0(5) 4_656 4_655
O1 Pr2 O4 64.3(4) 4_656 3_655
O1 Pr2 O4 59.8(4) 4_656 4_656
O1 Pr2 O4 72.8(4) 4_656 18_545
O1 Pr2 O5 74.5(4) 4_656 2_655
O1 Pr2 O5 52.3(3) 4_656 6_656
O2 Pr2 O2 77.2(5) 4_655 11_555
O2 Pr2 O3 63.7(3) 4_655 2_655
O2 Pr2 O3 53.7(4) 4_655 4_655
O2 Pr2 O4 80.2(4) 4_655 3_655
O2 Pr2 O4 142.7(5) 4_655 4_656
O2 Pr2 O4 71.4(4) 4_655 18_545
O2 Pr2 O5 104.3(5) 4_655 2_655
O2 Pr2 O5 162.4(5) 4_655 6_656
O2 Pr2 O3 97.5(6) 11_555 2_655
O2 Pr2 O3 128.5(6) 11_555 4_655
O2 Pr2 O4 136.6(7) 11_555 3_655
O2 Pr2 O4 65.9(4) 11_555 4_656
O2 Pr2 O4 77.9(5) 11_555 18_545
O2 Pr2 O5 165.2(8) 11_555 2_655
O2 Pr2 O5 112.6(5) 11_555 6_656
O3 Pr2 O3 50.0(3) 2_655 4_655
O3 Pr2 O4 105.1(4) 2_655 3_655
O3 Pr2 O4 124.8(5) 2_655 4_656
O3 Pr2 O4 134.7(4) 2_655 18_545
O3 Pr2 O5 70.9(4) 2_655 2_655
O3 Pr2 O5 99.7(4) 2_655 6_656
O3 Pr2 O4 55.4(3) 4_655 3_655
O3 Pr2 O4 162.6(5) 4_655 4_656
O3 Pr2 O4 98.0(4) 4_655 18_545
O3 Pr2 O5 50.6(3) 4_655 2_655
O3 Pr2 O5 111.7(4) 4_655 6_656
O4 Pr2 O4 123.3(5) 3_655 4_656
O4 Pr2 O4 59.9(4) 3_655 18_545
O4 Pr2 O5 57.3(3) 3_655 2_655
O4 Pr2 O5 99.7(3) 3_655 6_656
O4 Pr2 O4 94.7(4) 4_656 18_545
O4 Pr2 O5 112.7(5) 4_656 2_655
O4 Pr2 O5 51.0(3) 4_656 6_656
O4 Pr2 O5 116.7(6) 18_545 2_655
O4 Pr2 O5 124.0(4) 18_545 6_656
O5 Pr2 O5 62.4(3) 2_655 6_656
O5 Co1 O5 88.7(4) 1_555 2_555
O5 Co1 O5 88.7(6) 1_555 3_555
O5 Co1 O5 180.0(6) 1_555 4_556
O5 Co1 O5 91.3(5) 1_555 5_556
O5 Co1 O5 91.3(5) 1_555 6_556
O5 Co1 O5 88.7(6) 2_555 3_555
O5 Co1 O5 91.3(5) 2_555 4_556
O5 Co1 O5 180.0(6) 2_555 5_556
O5 Co1 O5 91.3(5) 2_555 6_556
O5 Co1 O5 91.3(5) 3_555 4_556
O5 Co1 O5 91.3(5) 3_555 5_556
O5 Co1 O5 180.0(7) 3_555 6_556
O5 Co1 O5 88.7(4) 4_556 5_556
O5 Co1 O5 88.7(6) 4_556 6_556
O5 Co1 O5 88.7(6) 5_556 6_556
O5 W1 O5 88.7(4) 1_555 2_555
O5 W1 O5 88.7(6) 1_555 3_555
O5 W1 O5 180.0(6) 1_555 4_556
O5 W1 O5 91.3(5) 1_555 5_556
O5 W1 O5 91.3(5) 1_555 6_556
O5 W1 O5 88.7(6) 2_555 3_555
O5 W1 O5 91.3(5) 2_555 4_556
O5 W1 O5 180.0(6) 2_555 5_556
O5 W1 O5 91.3(5) 2_555 6_556
O5 W1 O5 91.3(5) 3_555 4_556
O5 W1 O5 91.3(5) 3_555 5_556
O5 W1 O5 180.0(7) 3_555 6_556
O5 W1 O5 88.7(4) 4_556 5_556
O5 W1 O5 88.7(6) 4_556 6_556
O5 W1 O5 88.7(6) 5_556 6_556
O1 W2 O2 103.5(8) 1_555 1_555
O1 W2 O3 77.1(6) 1_555 1_555
O1 W2 O3 155.5(7) 1_555 5_555
O1 W2 O4 98.5(8) 1_555 1_555
O1 W2 O5 86.5(5) 1_555 3_555
O2 W2 O3 92.3(7) 1_555 1_555
O2 W2 O3 87.3(5) 1_555 5_555
O2 W2 O4 95.1(6) 1_555 1_555
O2 W2 O5 169.9(7) 1_555 3_555
O3 W2 O3 80.6(5) 1_555 5_555
O3 W2 O4 172.2(9) 1_555 1_555
O3 W2 O5 88.3(5) 1_555 3_555
O3 W2 O4 102.3(6) 5_555 1_555
O3 W2 O5 82.8(5) 5_555 3_555
O4 W2 O5 84.9(7) 1_555 3_555
Pr2 O1 Pr2 118.9(3) 3_665 4_656
Pr2 O1 W2 119.3(4) 3_665 1_555
Pr2 O1 O2 119.5(6) 3_665 1_555
Pr2 O1 O2 54.4(4) 3_665 10_555
Pr2 O1 O3 62.1(4) 3_665 1_555
Pr2 O1 O4 156.2(6) 3_665 1_555
Pr2 O1 O4 64.0(4) 3_665 6_556
Pr2 O1 O4 114.3(5) 3_665 9_555
Pr2 O1 O5 98.0(4) 3_665 3_555
Pr2 O1 O5 70.8(4) 3_665 5_556
Pr2 O1 W2 105.1(3) 4_656 1_555
Pr2 O1 O2 121.5(5) 4_656 1_555
Pr2 O1 O2 118.9(4) 4_656 10_555
Pr2 O1 O3 147.4(5) 4_656 1_555
Pr2 O1 O4 66.4(4) 4_656 1_555
Pr2 O1 O4 64.6(4) 4_656 6_556
Pr2 O1 O4 52.3(3) 4_656 9_555
Pr2 O1 O5 77.4(3) 4_656 3_555
Pr2 O1 O5 52.3(3) 4_656 5_556
W2 O1 O2 132.2(5) 1_555 10_555
W2 O1 O3 58.4(5) 1_555 1_555
W2 O1 O4 167.3(5) 1_555 6_556
W2 O1 O4 125.7(5) 1_555 9_555
W2 O1 O5 51.9(4) 1_555 3_555
W2 O1 O5 115.8(5) 1_555 5_556
O2 O1 O2 97.6(5) 1_555 10_555
O2 O1 O3 65.7(5) 1_555 1_555
O2 O1 O4 58.9(4) 1_555 1_555
O2 O1 O4 151.8(6) 1_555 6_556
O2 O1 O4 104.6(5) 1_555 9_555
O2 O1 O5 91.4(5) 1_555 3_555
O2 O1 O5 155.2(6) 1_555 5_556
O2 O1 O3 89.0(5) 10_555 1_555
O2 O1 O4 146.5(6) 10_555 1_555
O2 O1 O4 60.3(4) 10_555 6_556
O2 O1 O4 74.9(4) 10_555 9_555
O2 O1 O5 151.7(4) 10_555 3_555
O2 O1 O5 106.0(4) 10_555 5_556
O3 O1 O4 100.4(6) 1_555 1_555
O3 O1 O4 126.1(5) 1_555 6_556
O3 O1 O4 160.2(6) 1_555 9_555
O3 O1 O5 70.5(4) 1_555 3_555
O3 O1 O5 106.5(5) 1_555 5_556
O4 O1 O4 130.2(6) 1_555 6_556
O4 O1 O4 87.6(4) 1_555 9_555
O4 O1 O5 59.4(4) 1_555 3_555
O4 O1 O5 102.0(5) 1_555 5_556
O4 O1 O4 55.1(4) 6_556 9_555
O4 O1 O5 116.4(4) 6_556 3_555
O4 O1 O5 52.3(3) 6_556 5_556
O4 O1 O5 128.5(5) 9_555 3_555
O4 O1 O5 89.2(4) 9_555 5_556
O5 O1 O5 64.1(3) 3_555 5_556
Pr2 O2 Pr2 113.6(3) 4_655 12_445
Pr2 O2 W2 103.7(3) 4_655 1_555
Pr2 O2 O1 129.1(5) 4_655 1_555
Pr2 O2 O1 102.2(4) 4_655 10_555
Pr2 O2 O2 156.6(5) 4_655 9_555
Pr2 O2 O2 50.0(4) 4_655 14_544
Pr2 O2 O3 79.7(4) 4_655 1_555
Pr2 O2 O3 56.9(3) 4_655 5_555
Pr2 O2 O4 120.7(4) 4_655 1_555
Pr2 O2 O4 52.4(3) 4_655 9_554
Pr2 O2 O4 100.6(5) 4_655 14_544
Pr2 O2 W2 142.4(3) 12_445 1_555
Pr2 O2 O1 109.3(4) 12_445 1_555
Pr2 O2 O1 53.3(4) 12_445 10_555
Pr2 O2 O2 52.7(3) 12_445 9_555
Pr2 O2 O2 86.2(4) 12_445 14_544
Pr2 O2 O3 134.3(5) 12_445 1_555
Pr2 O2 O3 165.7(4) 12_445 5_555
Pr2 O2 O4 114.6(4) 12_445 1_555
Pr2 O2 O4 63.7(3) 12_445 9_554
Pr2 O2 O4 50.7(4) 12_445 14_544
W2 O2 O1 115.6(4) 1_555 10_555
W2 O2 O2 93.3(5) 1_555 9_555
W2 O2 O2 123.0(6) 1_555 14_544
W2 O2 O3 47.7(4) 1_555 1_555
W2 O2 O3 49.4(4) 1_555 5_555
W2 O2 O4 148.5(5) 1_555 9_554
W2 O2 O4 127.3(6) 1_555 14_544
O1 O2 O1 82.4(4) 1_555 10_555
O1 O2 O2 73.7(5) 1_555 9_555
O1 O2 O2 158.7(6) 1_555 14_544
O1 O2 O3 50.5(4) 1_555 1_555
O1 O2 O3 84.4(4) 1_555 5_555
O1 O2 O4 58.8(4) 1_555 1_555
O1 O2 O4 138.6(5) 1_555 9_554
O1 O2 O4 127.8(6) 1_555 14_544
O1 O2 O2 84.3(5) 10_555 9_555
O1 O2 O2 118.9(5) 10_555 14_544
O1 O2 O3 81.6(4) 10_555 1_555
O1 O2 O3 135.8(4) 10_555 5_555
O1 O2 O4 134.1(5) 10_555 1_555
O1 O2 O4 60.4(4) 10_555 9_554
O1 O2 O4 103.6(6) 10_555 14_544
O2 O2 O2 107.1(5) 9_555 14_544
O2 O2 O3 123.6(6) 9_555 1_555
O2 O2 O3 131.3(5) 9_555 5_555
O2 O2 O4 63.2(4) 9_555 1_555
O2 O2 O4 116.2(5) 9_555 9_554
O2 O2 O4 56.0(4) 9_555 14_544
O2 O2 O3 127.4(6) 14_544 1_555
O2 O2 O3 79.4(5) 14_544 5_555
O2 O2 O4 101.8(5) 14_544 1_555
O2 O2 O4 61.1(4) 14_544 9_554
O2 O2 O4 51.6(4) 14_544 14_544
O3 O2 O3 57.9(4) 1_555 5_555
O3 O2 O4 90.2(5) 1_555 1_555
O3 O2 O4 103.0(5) 1_555 9_554
O3 O2 O4 174.4(7) 1_555 14_544
O3 O2 O4 68.2(4) 5_555 1_555
O3 O2 O4 109.1(4) 5_555 9_554
O3 O2 O4 117.6(5) 5_555 14_544
O4 O2 O4 162.5(5) 1_555 9_554
O4 O2 O4 84.8(5) 1_555 14_544
O4 O2 O4 81.4(5) 9_554 14_544
Pr1 O3 Pr2 114.8(2) 1_555 3_665
Pr1 O3 Pr2 88.73(19) 1_555 4_655
Pr1 O3 W2 93.2(3) 1_555 1_555
Pr1 O3 W2 95.1(3) 1_555 6_555
Pr1 O3 O1 117.8(4) 1_555 1_555
Pr1 O3 O2 116.7(5) 1_555 1_555
Pr1 O3 O2 123.2(4) 1_555 6_555
Pr1 O3 O3 59.0(3) 1_555 5_555
Pr1 O3 O3 59.0(3) 1_555 6_555
Pr1 O3 O4 117.0(3) 1_555 6_555
Pr1 O3 O5 60.2(3) 1_555 1_555
Pr1 O3 O5 60.2(3) 1_555 3_555
Pr1 O3 O5 63.0(3) 1_555 5_555
Pr2 O3 Pr2 156.5(2) 3_665 4_655
Pr2 O3 W2 103.1(3) 3_665 1_555
Pr2 O3 W2 100.2(3) 3_665 6_555
Pr2 O3 O1 59.5(4) 3_665 1_555
Pr2 O3 O2 115.7(5) 3_665 1_555
Pr2 O3 O2 59.4(4) 3_665 6_555
Pr2 O3 O3 146.0(5) 3_665 5_555
Pr2 O3 O3 84.3(4) 3_665 6_555
Pr2 O3 O4 112.1(4) 3_665 6_555
Pr2 O3 O5 54.6(3) 3_665 1_555
Pr2 O3 O5 89.4(3) 3_665 3_555
Pr2 O3 O5 145.9(4) 3_665 5_555
Pr2 O3 W2 72.7(3) 4_655 1_555
Pr2 O3 W2 77.8(3) 4_655 6_555
Pr2 O3 O1 109.6(4) 4_655 1_555
Pr2 O3 O2 46.6(3) 4_655 1_555
Pr2 O3 O2 109.8(4) 4_655 6_555
Pr2 O3 O3 45.7(3) 4_655 5_555
Pr2 O3 O3 110.7(4) 4_655 6_555
Pr2 O3 O4 53.2(3) 4_655 6_555
Pr2 O3 O5 148.8(4) 4_655 1_555
Pr2 O3 O5 102.2(3) 4_655 3_555
Pr2 O3 O5 45.7(3) 4_655 5_555
W2 O3 W2 149.1(4) 1_555 6_555
W2 O3 O2 143.1(6) 1_555 6_555
W2 O3 O3 48.5(4) 1_555 5_555
W2 O3 O3 151.2(6) 1_555 6_555
W2 O3 O4 114.4(4) 1_555 6_555
W2 O3 O5 103.7(5) 1_555 1_555
W2 O3 O5 45.1(3) 1_555 3_555
W2 O3 O5 111.0(5) 1_555 5_555
W2 O3 O1 146.0(6) 6_555 1_555
W2 O3 O2 110.7(6) 6_555 1_555
W2 O3 O3 113.3(5) 6_555 5_555
W2 O3 O3 50.9(4) 6_555 6_555
W2 O3 O5 106.2(4) 6_555 1_555
W2 O3 O5 155.2(4) 6_555 3_555
W2 O3 O5 49.0(4) 6_555 5_555
O1 O3 O2 63.8(5) 1_555 1_555
O1 O3 O2 105.8(6) 1_555 6_555
O1 O3 O3 92.5(5) 1_555 5_555
O1 O3 O3 139.4(7) 1_555 6_555
O1 O3 O4 121.4(5) 1_555 6_555
O1 O3 O5 84.7(5) 1_555 1_555
O1 O3 O5 57.9(4) 1_555 3_555
O1 O3 O5 154.2(6) 1_555 5_555
O2 O3 O2 114.3(7) 1_555 6_555
O2 O3 O3 57.8(4) 1_555 5_555
O2 O3 O3 156.8(7) 1_555 6_555
O2 O3 O4 74.6(5) 1_555 6_555
O2 O3 O5 143.0(6) 1_555 1_555
O2 O3 O5 84.8(5) 1_555 3_555
O2 O3 O5 92.2(5) 1_555 5_555
O2 O3 O3 154.3(6) 6_555 5_555
O2 O3 O3 64.3(4) 6_555 6_555
O2 O3 O4 56.6(4) 6_555 6_555
O2 O3 O5 91.7(4) 6_555 1_555
O2 O3 O5 147.8(5) 6_555 3_555
O2 O3 O5 92.2(5) 6_555 5_555
O3 O3 O3 112.5(6) 5_555 6_555
O3 O3 O4 98.5(4) 5_555 6_555
O3 O3 O5 108.3(5) 5_555 1_555
O3 O3 O5 57.8(4) 5_555 3_555
O3 O3 O5 65.2(4) 5_555 5_555
O3 O3 O4 87.3(5) 6_555 6_555
O3 O3 O5 57.8(4) 6_555 1_555
O3 O3 O5 108.3(5) 6_555 3_555
O3 O3 O5 65.2(5) 6_555 5_555
O4 O3 O5 141.9(5) 6_555 1_555
O4 O3 O5 155.0(4) 6_555 3_555
O4 O3 O5 54.5(3) 6_555 5_555
O5 O3 O5 61.2(4) 1_555 3_555
O5 O3 O5 113.6(5) 1_555 5_555
O5 O3 O5 113.7(4) 3_555 5_555
Pr2 O4 Pr2 94.8(2) 2_545 4_656
Pr2 O4 Pr2 120.1(3) 2_545 17_555
Pr2 O4 W2 96.3(3) 2_545 1_555
Pr2 O4 O1 110.6(4) 2_545 1_555
Pr2 O4 O1 51.1(3) 2_545 5_556
Pr2 O4 O1 92.5(4) 2_545 14_544
Pr2 O4 O2 126.6(4) 2_545 1_555
Pr2 O4 O2 168.1(3) 2_545 9_555
Pr2 O4 O2 105.7(4) 2_545 14_545
Pr2 O4 O3 71.3(3) 2_545 5_555
Pr2 O4 O4 51.1(3) 2_545 16_545
Pr2 O4 O5 53.0(3) 2_545 3_555
Pr2 O4 Pr2 104.4(3) 4_656 17_555
Pr2 O4 W2 90.1(3) 4_656 1_555
Pr2 O4 O1 53.8(4) 4_656 1_555
Pr2 O4 O1 49.6(3) 4_656 5_556
Pr2 O4 O1 158.7(5) 4_656 14_544
Pr2 O4 O2 112.7(4) 4_656 1_555
Pr2 O4 O2 80.8(3) 4_656 9_555
Pr2 O4 O2 50.4(3) 4_656 14_545
Pr2 O4 O3 123.4(4) 4_656 5_555
Pr2 O4 O4 108.3(4) 4_656 16_545
Pr2 O4 O5 71.2(4) 4_656 3_555
Pr2 O4 W2 138.7(4) 17_555 1_555
Pr2 O4 O1 126.6(6) 17_555 1_555
Pr2 O4 O1 104.4(4) 17_555 5_556
Pr2 O4 O1 54.9(4) 17_555 14_544
Pr2 O4 O2 97.0(5) 17_555 1_555
Pr2 O4 O2 51.4(3) 17_555 9_555
Pr2 O4 O2 56.1(4) 17_555 14_545
Pr2 O4 O3 130.4(5) 17_555 5_555
Pr2 O4 O4 69.1(4) 17_555 16_545
Pr2 O4 O5 170.3(6) 17_555 3_555
W2 O4 O1 114.2(5) 1_555 5_556
W2 O4 O1 108.9(6) 1_555 14_544
W2 O4 O2 94.8(5) 1_555 9_555
W2 O4 O2 135.4(6) 1_555 14_545
W2 O4 O4 142.5(6) 1_555 16_545
W2 O4 O5 50.9(5) 1_555 3_555
O1 O4 O1 94.3(5) 1_555 5_556
O1 O4 O1 140.3(7) 1_555 14_544
O1 O4 O2 62.2(5) 1_555 1_555
O1 O4 O2 75.8(5) 1_555 9_555
O1 O4 O2 96.3(6) 1_555 14_545
O1 O4 O3 79.7(5) 1_555 5_555
O1 O4 O4 156.4(6) 1_555 16_545
O1 O4 O5 58.3(4) 1_555 3_555
O1 O4 O1 124.9(5) 5_556 14_544
O1 O4 O2 155.1(5) 5_556 1_555
O1 O4 O2 119.7(4) 5_556 9_555
O1 O4 O2 59.3(4) 5_556 14_545
O1 O4 O3 115.6(5) 5_556 5_555
O1 O4 O4 62.9(4) 5_556 16_545
O1 O4 O5 66.1(5) 5_556 3_555
O1 O4 O2 78.1(5) 14_544 1_555
O1 O4 O2 88.1(4) 14_544 9_555
O1 O4 O2 108.3(5) 14_544 14_545
O1 O4 O3 77.9(5) 14_544 5_555
O1 O4 O4 62.0(4) 14_544 16_545
O1 O4 O5 128.2(6) 14_544 3_555
O2 O4 O2 65.2(4) 1_555 9_555
O2 O4 O2 127.3(6) 1_555 14_545
O2 O4 O3 55.2(4) 1_555 5_555
O2 O4 O4 138.8(5) 1_555 16_545
O2 O4 O5 92.7(5) 1_555 3_555
O2 O4 O2 62.9(4) 9_555 14_545
O2 O4 O3 120.4(5) 9_555 5_555
O2 O4 O4 119.7(4) 9_555 16_545
O2 O4 O5 134.0(6) 9_555 3_555
O2 O4 O3 173.5(6) 14_545 5_555
O2 O4 O4 78.0(4) 14_545 16_545
O2 O4 O5 116.9(6) 14_545 3_555
O3 O4 O4 103.7(5) 5_555 16_545
O3 O4 O5 56.6(4) 5_555 3_555
O4 O4 O5 103.6(6) 16_545 3_555
Pr1 O5 Pr2 109.0(2) 1_555 3_665
Pr1 O5 Pr2 154.1(2) 1_555 5_566
Pr1 O5 Co1 88.2(2) 1_555 1_555
Pr1 O5 W1 88.2(2) 1_555 1_555
Pr1 O5 W2 89.6(3) 1_555 2_555
Pr1 O5 O1 105.9(5) 1_555 2_555
Pr1 O5 O1 160.0(4) 1_555 6_556
Pr1 O5 O3 54.5(3) 1_555 1_555
Pr1 O5 O3 54.5(3) 1_555 2_555
Pr1 O5 O3 56.7(3) 1_555 6_555
Pr1 O5 O4 125.0(4) 1_555 2_555
Pr1 O5 O5 57.8(2) 1_555 2_555
Pr1 O5 O5 57.8(3) 1_555 3_555
Pr1 O5 O5 118.5(3) 1_555 5_556
Pr1 O5 O5 118.5(3) 1_555 6_556
Pr2 O5 Pr2 96.2(2) 3_665 5_566
Pr2 O5 Co1 110.7(2) 3_665 1_555
Pr2 O5 W1 110.7(2) 3_665 1_555
Pr2 O5 W2 105.5(3) 3_665 2_555
Pr2 O5 O1 131.1(4) 3_665 2_555
Pr2 O5 O1 53.2(3) 3_665 6_556
Pr2 O5 O3 54.5(3) 3_665 1_555
Pr2 O5 O3 140.6(4) 3_665 2_555
Pr2 O5 O3 83.7(4) 3_665 6_555
Pr2 O5 O4 69.7(4) 3_665 2_555
Pr2 O5 O5 148.0(3) 3_665 2_555
Pr2 O5 O5 88.1(3) 3_665 3_555
Pr2 O5 O5 70.4(3) 3_665 5_556
Pr2 O5 O5 121.7(3) 3_665 6_556
Pr2 O5 Co1 88.6(2) 5_566 1_555
Pr2 O5 W1 88.6(2) 5_566 1_555
Pr2 O5 W2 77.5(3) 5_566 2_555
Pr2 O5 O1 50.2(4) 5_566 2_555
Pr2 O5 O1 45.7(3) 5_566 6_556
Pr2 O5 O3 150.4(4) 5_566 1_555
Pr2 O5 O3 101.7(3) 5_566 2_555
Pr2 O5 O3 122.6(4) 5_566 6_555
Pr2 O5 O4 57.9(3) 5_566 2_555
Pr2 O5 O5 103.1(3) 5_566 2_555
Pr2 O5 O5 131.3(4) 5_566 3_555
Pr2 O5 O5 75.2(3) 5_566 5_556
Pr2 O5 O5 47.2(3) 5_566 6_556
Co1 O5 W2 142.4(3) 1_555 2_555
Co1 O5 O1 103.6(5) 1_555 2_555
Co1 O5 O1 90.4(4) 1_555 6_556
Co1 O5 O3 104.6(4) 1_555 1_555
Co1 O5 O3 104.6(4) 1_555 2_555
Co1 O5 O3 144.9(5) 1_555 6_555
Co1 O5 O4 145.6(5) 1_555 2_555
Co1 O5 O5 45.7(3) 1_555 2_555
Co1 O5 O5 45.7(3) 1_555 3_555
W1 O5 W2 142.4(3) 1_555 2_555
W1 O5 O1 103.6(5) 1_555 2_555
W1 O5 O1 90.4(4) 1_555 6_556
W1 O5 O3 104.6(4) 1_555 1_555
W1 O5 O3 104.6(4) 1_555 2_555
W1 O5 O3 144.9(5) 1_555 6_555
W1 O5 O4 145.6(5) 1_555 2_555
W1 O5 O5 45.7(3) 1_555 2_555
W1 O5 O5 45.7(3) 1_555 3_555
W2 O5 O1 103.4(4) 2_555 6_556
W2 O5 O3 104.5(5) 2_555 1_555
W2 O5 O3 46.6(3) 2_555 2_555
W2 O5 O3 48.2(4) 2_555 6_555
W2 O5 O5 103.4(4) 2_555 2_555
W2 O5 O5 147.3(5) 2_555 3_555
W2 O5 O5 151.7(5) 2_555 5_556
W2 O5 O5 106.5(4) 2_555 6_556
O1 O5 O1 93.9(5) 2_555 6_556
O1 O5 O3 144.7(6) 2_555 1_555
O1 O5 O3 51.6(4) 2_555 2_555
O1 O5 O3 87.8(5) 2_555 6_555
O1 O5 O4 62.3(4) 2_555 2_555
O1 O5 O5 80.4(5) 2_555 2_555
O1 O5 O5 140.1(7) 2_555 3_555
O1 O5 O5 119.4(6) 2_555 5_556
O1 O5 O5 65.1(4) 2_555 6_556
O1 O5 O3 106.8(5) 6_556 1_555
O1 O5 O3 144.5(5) 6_556 2_555
O1 O5 O3 122.3(5) 6_556 6_555
O1 O5 O4 61.6(4) 6_556 2_555
O1 O5 O5 131.0(4) 6_556 2_555
O1 O5 O5 108.4(5) 6_556 3_555
O1 O5 O5 50.8(3) 6_556 5_556
O1 O5 O5 72.7(3) 6_556 6_556
O3 O5 O3 100.4(4) 1_555 2_555
O3 O5 O3 57.0(4) 1_555 6_555
O3 O5 O4 102.6(6) 1_555 2_555
O3 O5 O5 105.0(4) 1_555 2_555
O3 O5 O5 59.4(4) 1_555 3_555
O3 O5 O5 95.7(4) 1_555 5_556
O3 O5 O5 148.1(5) 1_555 6_556
O3 O5 O3 57.0(3) 2_555 6_555
O3 O5 O4 90.7(4) 2_555 2_555
O3 O5 O5 59.4(3) 2_555 2_555
O3 O5 O5 105.0(5) 2_555 3_555
O3 O5 O5 148.2(5) 2_555 5_556
O3 O5 O5 95.7(4) 2_555 6_556
O3 O5 O4 68.9(4) 6_555 2_555
O3 O5 O5 106.1(4) 6_555 2_555
O3 O5 O5 106.1(5) 6_555 3_555
O3 O5 O5 150.7(5) 6_555 5_556
O3 O5 O5 150.8(5) 6_555 6_556
O4 O5 O5 142.2(5) 2_555 2_555
O4 O5 O5 157.5(6) 2_555 3_555
O4 O5 O5 112.4(5) 2_555 5_556
O4 O5 O5 104.5(4) 2_555 6_556
O5 O5 O5 60.0(4) 2_555 3_555
O5 O5 O5 90.0(4) 2_555 5_556
O5 O5 O5 60.8(3) 2_555 6_556
O5 O5 O5 60.8(4) 3_555 5_556
O5 O5 O5 90.0(4) 3_555 6_556
O5 O5 O5 58.5(4) 5_556 6_556

#=============================================================================

# STRUCTURE FACTORS :

